# Electronic Supplementary Material (ESI) for CrystEngComm.
# This journal is © The Royal Society of Chemistry 2017

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_complex3
_database_code_depnum_ccdc_archive 'CCDC 1514243'
_audit_update_record             
;
2016-12-27 deposited with the CCDC.
2017-04-28 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C14 H36 Mn2 Mo6 N4 O36 Te'
_chemical_formula_weight         1649.59

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Triclinic
_symmetry_space_group_name_H-M   'P -1'

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   9.9460(4)
_cell_length_b                   10.7000(5)
_cell_length_c                   10.8400(5)
_cell_angle_alpha                97.0350(10)
_cell_angle_beta                 99.1390(10)
_cell_angle_gamma                116.0830(10)
_cell_volume                     998.63(8)
_cell_formula_units_Z            1
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    4566
_cell_measurement_theta_min      2.1708
_cell_measurement_theta_max      28.3344

_exptl_crystal_description       BLOCK
_exptl_crystal_colour            YELLOW
_exptl_crystal_size_max          0.35
_exptl_crystal_size_mid          0.28
_exptl_crystal_size_min          0.20
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    2.743
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             790
_exptl_absorpt_coefficient_mu    3.268
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.347
_exptl_absorpt_correction_T_max  0.520
_exptl_absorpt_process_details   SADABS

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            7434
_diffrn_reflns_av_R_equivalents  0.0127
_diffrn_reflns_av_sigmaI/netI    0.0233
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_theta_min         1.95
_diffrn_reflns_theta_max         28.35
_reflns_number_total             4992
_reflns_number_gt                4494
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'SMART (Bruker, 2001)'
_computing_cell_refinement       'SMART (Bruker, 2001)'
_computing_data_reduction        'SAINT+ (Bruker, 1999)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_molecular_graphics    'PLATON (Spek, 2003)'
_computing_publication_material  'SHELXTL (1998)'

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0308P)²+2.7639P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         4959
_refine_ls_number_parameters     286
_refine_ls_number_restraints     6
_refine_ls_R_factor_all          0.0276
_refine_ls_R_factor_gt           0.0240
_refine_ls_wR_factor_ref         0.0642
_refine_ls_wR_factor_gt          0.0622
_refine_ls_goodness_of_fit_ref   0.998
_refine_ls_restrained_S_all      0.999
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Te1 Te 0.0000 0.0000 0.5000 0.00830(6) Uani 1 2 d S . .
Mo1 Mo 0.16785(3) -0.02714(3) 0.26504(2) 0.01271(6) Uani 1 1 d . . .
Mn1 Mn -0.38151(5) 0.35280(5) 0.60828(5) 0.01408(10) Uani 1 1 d . . .
O1 O -0.2062(3) 0.3007(3) 0.5767(2) 0.0232(5) Uani 1 1 d . . .
N1 N -0.6340(4) 0.3314(4) 1.0883(3) 0.0362(8) Uani 1 1 d . . .
H1B H -0.6469 0.3647 1.1592 0.043 Uiso 1 1 calc R . .
O1W O -0.4527(3) 0.3388(3) 0.4014(2) 0.0205(5) Uani 1 1 d . . .
H1WA H -0.4394 0.4101 0.3683 0.025 Uiso 1 1 d R . .
H1WB H -0.5288 0.2657 0.3516 0.025 Uiso 1 1 d R . .
C1 C -0.7599(4) 0.2365(4) 0.9919(4) 0.0265(8) Uani 1 1 d . . .
H1A H -0.8593 0.2074 1.0030 0.032 Uiso 1 1 calc R . .
Mo2 Mo 0.09714(3) 0.24642(3) 0.33004(2) 0.01183(6) Uani 1 1 d . . .
O2 O -0.2978(3) 0.3730(3) 0.8141(2) 0.0239(5) Uani 1 1 d . . .
N2 N -0.1983(3) 0.3856(4) 1.0188(3) 0.0261(7) Uani 1 1 d . . .
H2B H -0.2145 0.3791 1.0939 0.031 Uiso 1 1 calc R . .
C2 C -0.7370(3) 0.1865(3) 0.8818(3) 0.0148(6) Uani 1 1 d . . .
H2A H -0.8225 0.1220 0.8174 0.018 Uiso 1 1 calc R . .
O2W O -0.5713(3) 0.3962(3) 0.6368(2) 0.0209(5) Uani 1 1 d . . .
H2WB H -0.6651 0.3364 0.6289 0.025 Uiso 1 1 d R . .
H23 H -0.6474 0.3438 0.5693 0.025 Uiso 1 1 d R . .
Mo3 Mo -0.03748(3) 0.28795(3) 0.58290(3) 0.01365(7) Uani 1 1 d . . .
C3 C -0.5967(4) 0.2254(4) 0.8605(3) 0.0213(7) Uani 1 1 d . . .
H3A H -0.5865 0.1886 0.7823 0.026 Uiso 1 1 calc R . .
O3W O -0.5330(3) 0.1267(3) 0.5943(2) 0.0235(5) Uani 1 1 d . . .
H3WA H -0.6219 0.0625 0.5523 0.028 Uiso 1 1 d R . .
H3WB H -0.4993 0.0916 0.6502 0.028 Uiso 1 1 d R . .
C4 C -0.4671(3) 0.3200(4) 0.9542(3) 0.0180(6) Uani 1 1 d . . .
O4W O -0.3422(6) 0.0412(5) 1.0220(5) 0.0887(16) Uani 1 1 d U . .
H4WA H -0.2958 0.1089 1.0879 0.106 Uiso 1 1 d R . .
H4WB H -0.2744 0.0363 0.9858 0.106 Uiso 1 1 d R . .
O5W O -0.3134(4) 0.2426(4) 1.2333(3) 0.0462(8) Uani 1 1 d . . .
H5WA H -0.3180 0.3185 1.2596 0.055 Uiso 1 1 d R . .
H5WB H -0.2477 0.2372 1.2900 0.055 Uiso 1 1 d R . .
C5 C -0.4862(4) 0.3735(4) 1.0707(3) 0.0218(7) Uani 1 1 d . . .
H5A H -0.4007 0.4366 1.1359 0.026 Uiso 1 1 calc R . .
O6 O -0.0221(3) 0.2221(2) 0.7371(2) 0.0162(4) Uani 1 1 d . . .
C6 C -0.3136(4) 0.3622(4) 0.9238(3) 0.0191(6) Uani 1 1 d . . .
O7 O 0.1042(3) -0.0375(3) 0.1067(2) 0.0252(5) Uani 1 1 d . . .
C7 C -0.0433(4) 0.4222(4) 1.0003(4) 0.0259(8) Uani 1 1 d . . .
H7A H -0.0514 0.3656 0.9197 0.039 Uiso 1 1 calc R . .
H7B H 0.0126 0.4002 1.0685 0.039 Uiso 1 1 calc R . .
O8 O -0.1667(2) 0.0375(2) 0.5273(2) 0.0117(4) Uani 1 1 d . . .
O9 O -0.0607(3) 0.2614(2) 0.3964(2) 0.0170(5) Uani 1 1 d . . .
O10 O -0.0320(2) 0.0107(2) 0.32177(19) 0.0116(4) Uani 1 1 d . . .
O11 O 0.2480(2) 0.1747(2) 0.3269(2) 0.0146(4) Uani 1 1 d . . .
O12 O -0.1245(2) -0.2042(2) 0.4637(2) 0.0119(4) Uani 1 1 d . . .
O13 O 0.2405(3) 0.4228(2) 0.3711(2) 0.0213(5) Uani 1 1 d . . .
O14 O 0.1104(3) 0.4558(3) 0.6337(3) 0.0291(6) Uani 1 1 d . . .
O15 O 0.0171(3) 0.2143(3) 0.1716(2) 0.0223(5) Uani 1 1 d . . .
O17 O 0.3399(3) -0.0321(3) 0.2790(3) 0.0250(5) Uani 1 1 d . . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Te1 O8 1.926(2) . ?
Te1 O8 1.926(2) 2_556 ?
Te1 O12 1.928(2) 2_556 ?
Te1 O12 1.928(2) . ?
Te1 O10 1.933(2) . ?
Te1 O10 1.933(2) 2_556 ?
Mo1 O7 1.704(2) . ?
Mo1 O17 1.719(2) . ?
Mo1 O11 1.926(2) . ?
Mo1 O6 1.942(2) 2_556 ?
Mo1 O8 2.268(2) 2_556 ?
Mo1 O10 2.351(2) . ?
Mn1 O1 2.114(2) . ?
Mn1 O13 2.143(2) 2_566 ?
Mn1 O3W 2.186(2) . ?
Mn1 O2W 2.191(2) . ?
Mn1 O2 2.203(2) . ?
Mn1 O1W 2.207(2) . ?
O1 Mo3 1.733(2) . ?
N1 C1 1.377(5) . ?
N1 C5 1.388(5) . ?
C1 C2 1.342(5) . ?
Mo2 O15 1.697(2) . ?
Mo2 O13 1.737(2) . ?
Mo2 O9 1.887(2) . ?
Mo2 O11 1.966(2) . ?
Mo2 O10 2.254(2) . ?
Mo2 O12 2.332(2) 2_556 ?
O2 C6 1.236(4) . ?
N2 C6 1.322(4) . ?
N2 C7 1.468(4) . ?
C2 C3 1.337(4) . ?
Mo3 O14 1.694(3) . ?
Mo3 O6 1.902(2) . ?
Mo3 O9 1.968(2) . ?
Mo3 O12 2.252(2) 2_556 ?
Mo3 O8 2.350(2) . ?
C3 C4 1.380(5) . ?
C4 C5 1.397(5) . ?
C4 C6 1.494(4) . ?
O6 Mo1 1.942(2) 2_556 ?
C7 C7 1.502(7) 2_567 ?
O8 Mo1 2.269(2) 2_556 ?
O12 Mo3 2.252(2) 2_556 ?
O12 Mo2 2.332(2) 2_556 ?
O13 Mn1 2.143(2) 2_566 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O8 Te1 O8 180.00(3) . 2_556 ?
O8 Te1 O12 85.97(9) . 2_556 ?
O8 Te1 O12 94.03(9) 2_556 2_556 ?
O8 Te1 O12 94.03(9) . . ?
O8 Te1 O12 85.97(9) 2_556 . ?
O12 Te1 O12 180.0 2_556 . ?
O8 Te1 O10 94.04(9) . . ?
O8 Te1 O10 85.96(9) 2_556 . ?
O12 Te1 O10 86.15(9) 2_556 . ?
O12 Te1 O10 93.85(9) . . ?
O8 Te1 O10 85.96(9) . 2_556 ?
O8 Te1 O10 94.04(9) 2_556 2_556 ?
O12 Te1 O10 93.85(9) 2_556 2_556 ?
O12 Te1 O10 86.15(9) . 2_556 ?
O10 Te1 O10 180.0 . 2_556 ?
O7 Mo1 O17 105.79(13) . . ?
O7 Mo1 O11 98.90(11) . . ?
O17 Mo1 O11 98.53(11) . . ?
O7 Mo1 O6 95.18(11) . 2_556 ?
O17 Mo1 O6 103.13(11) . 2_556 ?
O11 Mo1 O6 149.81(9) . 2_556 ?
O7 Mo1 O8 160.46(10) . 2_556 ?
O17 Mo1 O8 92.70(10) . 2_556 ?
O11 Mo1 O8 84.21(9) . 2_556 ?
O6 Mo1 O8 74.09(8) 2_556 2_556 ?
O7 Mo1 O10 93.03(11) . . ?
O17 Mo1 O10 160.27(10) . . ?
O11 Mo1 O10 72.20(8) . . ?
O6 Mo1 O10 80.54(8) 2_556 . ?
O8 Mo1 O10 69.42(7) 2_556 . ?
O1 Mn1 O13 94.26(10) . 2_566 ?
O1 Mn1 O3W 88.65(10) . . ?
O13 Mn1 O3W 176.73(10) 2_566 . ?
O1 Mn1 O2W 177.26(10) . . ?
O13 Mn1 O2W 88.32(9) 2_566 . ?
O3W Mn1 O2W 88.80(9) . . ?
O1 Mn1 O2 87.61(10) . . ?
O13 Mn1 O2 90.19(10) 2_566 . ?
O3W Mn1 O2 88.43(10) . . ?
O2W Mn1 O2 93.30(9) . . ?
O1 Mn1 O1W 90.23(9) . . ?
O13 Mn1 O1W 87.89(9) 2_566 . ?
O3W Mn1 O1W 93.60(9) . . ?
O2W Mn1 O1W 88.95(9) . . ?
O2 Mn1 O1W 177.00(9) . . ?
Mo3 O1 Mn1 166.72(16) . . ?
C1 N1 C5 120.0(3) . . ?
C2 C1 N1 119.0(3) . . ?
O15 Mo2 O13 105.97(12) . . ?
O15 Mo2 O9 98.88(11) . . ?
O13 Mo2 O9 101.25(11) . . ?
O15 Mo2 O11 101.64(11) . . ?
O13 Mo2 O11 92.30(10) . . ?
O9 Mo2 O11 151.20(9) . . ?
O15 Mo2 O10 88.95(10) . . ?
O13 Mo2 O10 161.57(10) . . ?
O9 Mo2 O10 86.70(9) . . ?
O11 Mo2 O10 73.77(8) . . ?
O15 Mo2 O12 157.66(10) . 2_556 ?
O13 Mo2 O12 96.09(10) . 2_556 ?
O9 Mo2 O12 72.83(8) . 2_556 ?
O11 Mo2 O12 80.62(8) . 2_556 ?
O10 Mo2 O12 70.18(7) . 2_556 ?
C6 O2 Mn1 154.3(2) . . ?
C6 N2 C7 122.2(3) . . ?
C3 C2 C1 123.0(3) . . ?
O14 Mo3 O1 106.95(13) . . ?
O14 Mo3 O6 99.11(12) . . ?
O1 Mo3 O6 100.13(11) . . ?
O14 Mo3 O9 101.06(12) . . ?
O1 Mo3 O9 93.72(11) . . ?
O6 Mo3 O9 150.97(9) . . ?
O14 Mo3 O12 90.92(11) . 2_556 ?
O1 Mo3 O12 159.85(11) . 2_556 ?
O6 Mo3 O12 85.75(9) . 2_556 ?
O9 Mo3 O12 73.31(8) . 2_556 ?
O14 Mo3 O8 159.12(11) . . ?
O1 Mo3 O8 93.56(10) . . ?
O6 Mo3 O8 72.82(8) . . ?
O9 Mo3 O8 81.01(9) . . ?
O12 Mo3 O8 69.59(7) 2_556 . ?
C2 C3 C4 120.2(3) . . ?
C3 C4 C5 118.6(3) . . ?
C3 C4 C6 117.7(3) . . ?
C5 C4 C6 123.7(3) . . ?
N1 C5 C4 119.4(3) . . ?
Mo3 O6 Mo1 117.62(11) . 2_556 ?
O2 C6 N2 122.5(3) . . ?
O2 C6 C4 120.7(3) . . ?
N2 C6 C4 116.8(3) . . ?
N2 C7 C7 110.6(4) . 2_567 ?
Te1 O8 Mo1 103.88(9) . 2_556 ?
Te1 O8 Mo3 100.45(8) . . ?
Mo1 O8 Mo3 90.75(7) 2_556 . ?
Mo2 O9 Mo3 117.77(11) . . ?
Te1 O10 Mo2 103.12(9) . . ?
Te1 O10 Mo1 100.71(9) . . ?
Mo2 O10 Mo1 92.24(7) . . ?
Mo1 O11 Mo2 117.06(10) . . ?
Te1 O12 Mo3 103.92(9) . 2_556 ?
Te1 O12 Mo2 100.50(9) . 2_556 ?
Mo3 O12 Mo2 92.08(8) 2_556 2_556 ?
Mo2 O13 Mn1 167.15(15) . 2_566 ?

_diffrn_measured_fraction_theta_max 0.994
_diffrn_reflns_theta_full        28.35
_diffrn_measured_fraction_theta_full 0.994
_refine_diff_density_max         1.003
_refine_diff_density_min         -0.938
_refine_diff_density_rms         0.128
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_complex3
_database_code_depnum_ccdc_archive 'CCDC 1514244'
_audit_update_record             
;
2016-12-27 deposited with the CCDC.
2017-04-28 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C18 H25 Cr Mn2 Mo6 N14 O28'
_chemical_formula_weight         1623.04

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cr Cr 0.3209 0.6236 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Triclinic
_symmetry_space_group_name_H-M   'P -1'

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   7.1060(13)
_cell_length_b                   11.066(2)
_cell_length_c                   13.489(2)
_cell_angle_alpha                86.196(3)
_cell_angle_beta                 79.701(3)
_cell_angle_gamma                89.749(3)
_cell_volume                     1041.3(3)
_cell_formula_units_Z            1
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    5005
_cell_measurement_theta_min      2.3216
_cell_measurement_theta_max      28.3763

_exptl_crystal_description       BLOCK
_exptl_crystal_colour            YELLOW
_exptl_crystal_size_max          0.40
_exptl_crystal_size_mid          0.35
_exptl_crystal_size_min          0.26
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    2.588
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             776
_exptl_absorpt_coefficient_mu    2.691
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.354
_exptl_absorpt_correction_T_max  0.497
_exptl_absorpt_process_details   SADABS

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            6840
_diffrn_reflns_av_R_equivalents  0.0133
_diffrn_reflns_av_sigmaI/netI    0.0264
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_theta_min         1.84
_diffrn_reflns_theta_max         28.38
_reflns_number_total             5221
_reflns_number_gt                4630
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'SMART (Bruker, 2001)'
_computing_cell_refinement       'SMART (Bruker, 2001)'
_computing_data_reduction        'SAINT+ (Bruker, 1999)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_molecular_graphics    'PLATON (Spek, 2003)'
_computing_publication_material  'SHELXTL (1998)'

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0475P)²+10.8290P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    mixed
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         5025
_refine_ls_number_parameters     317
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0392
_refine_ls_R_factor_gt           0.0359
_refine_ls_wR_factor_ref         0.1065
_refine_ls_wR_factor_gt          0.1043
_refine_ls_goodness_of_fit_ref   1.003
_refine_ls_restrained_S_all      1.003
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 1.00513(6) 0.15941(3) 0.27981(3) 0.01231(10) Uani 1 1 d . . .
Cr1 Cr 1.0000 0.0000 0.5000 0.00925(19) Uani 1 2 d S . .
N1 N 0.4173(6) 0.5485(4) 0.2957(4) 0.0204(9) Uani 1 1 d . . .
O1 O 0.8321(5) 0.2478(3) 0.2350(3) 0.0215(8) Uani 1 1 d . . .
O2 O 0.4487(5) 0.2711(3) 0.3417(3) 0.0219(8) Uani 1 1 d . . .
Mo2 Mo 0.72387(5) -0.09259(4) 0.34439(3) 0.01209(10) Uani 1 1 d . . .
C2 C 0.5254(9) 0.1962(7) -0.0795(5) 0.0402(17) Uani 1 1 d . . .
H2A H 0.4005 0.1999 -0.0915 0.048 Uiso 1 1 calc R . .
O2W O 0.8332(6) 0.5318(4) 0.1597(4) 0.0333(10) Uani 1 1 d . . .
H2WA H 0.8428 0.6003 0.1835 0.040 Uiso 1 1 d R . .
H2WB H 0.9449 0.5104 0.1331 0.040 Uiso 1 1 d R . .
Mo3 Mo 0.73282(6) -0.24694(3) 0.55542(3) 0.01330(10) Uani 1 1 d . . .
N3 N 0.1395(7) 0.6193(4) 0.2638(4) 0.0244(10) Uani 1 1 d . . .
O3 O 0.9360(5) -0.0028(3) 0.2554(3) 0.0153(7) Uani 1 1 d . . .
O3W O 0.7678(7) 0.4289(4) 0.3863(4) 0.0346(11) Uani 1 1 d . . .
H3WA H 0.8464 0.3758 0.4017 0.042 Uiso 1 1 d R . .
H3WB H 0.7364 0.4716 0.4367 0.042 Uiso 1 1 d R . .
C3 C 0.6559(11) 0.1231(8) -0.1341(6) 0.0456(19) Uani 1 1 d . . .
H3A H 0.6177 0.0757 -0.1815 0.055 Uiso 1 1 calc R . .
C4 C 0.3494(8) 0.6321(5) 0.3603(4) 0.0231(11) Uani 1 1 d . . .
H22 H 0.406(10) 0.649(6) 0.414(5) 0.025(17) Uiso 1 1 d . . .
Mn4 Mn 0.64439(11) 0.40474(7) 0.25693(6) 0.01710(16) Uani 1 1 d . . .
N4 N 0.4704(6) 0.3989(4) 0.1326(3) 0.0164(8) Uani 1 1 d . . .
O4 O 0.8050(4) 0.0736(3) 0.4240(2) 0.0113(6) Uani 1 1 d . . .
O5 O 0.9394(5) -0.1485(3) 0.4377(2) 0.0128(6) Uani 1 1 d . . .
N5 N 0.8355(8) 0.1192(5) -0.1200(4) 0.0302(11) Uani 1 1 d . . .
C5 C 0.2818(7) 0.5432(5) 0.2377(4) 0.0181(9) Uani 1 1 d . . .
N6 N 0.2773(7) 0.3740(5) 0.0218(4) 0.0274(10) Uani 1 1 d . . .
H6B H 0.2341 0.3486 -0.0288 0.033 Uiso 1 1 calc R . .
O6 O 0.7509(6) -0.2194(4) 0.2794(3) 0.0251(8) Uani 1 1 d . . .
C6 C 0.7685(8) 0.2587(6) 0.0068(5) 0.0281(12) Uani 1 1 d . . .
H6A H 0.8101 0.3040 0.0545 0.034 Uiso 1 1 calc R . .
O7 O 1.1994(5) 0.1699(4) 0.1864(3) 0.0229(8) Uani 1 1 d . . .
N7 N 0.1902(7) 0.4520(4) 0.0894(4) 0.0241(10) Uani 1 1 d . . .
C7 C 0.3086(7) 0.4645(4) 0.1540(4) 0.0181(9) Uani 1 1 d . . .
N8 N 0.1846(7) 0.6771(4) 0.3428(4) 0.0249(10) Uani 1 1 d . . .
C8 C 0.5796(8) 0.2648(5) -0.0063(4) 0.0205(10) Uani 1 1 d . . .
O9 O 0.5801(5) -0.1498(3) 0.4753(3) 0.0163(7) Uani 1 1 d . . .
C9 C 0.4427(7) 0.3453(5) 0.0501(4) 0.0185(9) Uani 1 1 d . . .
O10 O 0.8130(4) -0.0669(3) 0.6161(2) 0.0118(6) Uani 1 1 d . . .
C10 C 0.8949(10) 0.1852(7) -0.0513(5) 0.0368(15) Uani 1 1 d . . .
H10A H 1.0218 0.1814 -0.0427 0.044 Uiso 1 1 calc R . .
O11 O 0.7514(6) -0.3777(4) 0.4953(3) 0.0283(9) Uani 1 1 d . . .
O12 O 0.5316(5) -0.0199(4) 0.3069(3) 0.0232(8) Uani 1 1 d . . .
O13 O 1.0530(5) 0.2743(3) 0.3742(3) 0.0172(7) Uani 1 1 d . . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O7 1.693(4) . ?
Mo1 O1 1.735(4) . ?
Mo1 O3 1.928(3) . ?
Mo1 O13 1.930(4) . ?
Mo1 O10 2.266(3) 2_756 ?
Mo1 O4 2.342(3) . ?
Cr1 O10 1.969(3) 2_756 ?
Cr1 O10 1.969(3) . ?
Cr1 O5 1.977(3) . ?
Cr1 O5 1.977(3) 2_756 ?
Cr1 O4 2.005(3) . ?
Cr1 O4 2.005(3) 2_756 ?
N1 C4 1.342(7) . ?
N1 C5 1.348(7) . ?
N1 Mn4 2.279(4) . ?
O1 Mn4 2.189(4) . ?
O2 Mo3 1.725(4) 2_656 ?
O2 Mn4 2.157(4) . ?
Mo2 O6 1.695(4) . ?
Mo2 O12 1.718(4) . ?
Mo2 O9 1.942(4) . ?
Mo2 O3 1.977(3) . ?
Mo2 O5 2.211(3) . ?
Mo2 O4 2.315(3) . ?
C2 C3 1.373(9) . ?
C2 C8 1.392(8) . ?
O2W Mn4 2.154(4) . ?
Mo3 O11 1.699(4) . ?
Mo3 O2 1.725(4) 2_656 ?
Mo3 O9 1.938(3) . ?
Mo3 O13 1.945(3) 2_756 ?
Mo3 O5 2.194(3) . ?
Mo3 O10 2.315(3) . ?
N3 C5 1.326(6) . ?
N3 N8 1.365(6) . ?
O3W Mn4 2.121(4) . ?
C3 N5 1.324(9) . ?
C4 N8 1.324(7) . ?
Mn4 N4 2.259(4) . ?
N4 C9 1.341(6) . ?
N4 C7 1.354(6) . ?
N5 C10 1.343(8) . ?
C5 C7 1.457(7) . ?
N6 C9 1.330(7) . ?
N6 N7 1.362(6) . ?
C6 C10 1.382(8) . ?
C6 C8 1.386(8) . ?
N7 C7 1.328(7) . ?
C8 C9 1.461(7) . ?
O10 Mo1 2.266(3) 2_756 ?
O13 Mo3 1.945(3) 2_756 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O7 Mo1 O1 105.31(19) . . ?
O7 Mo1 O3 95.39(17) . . ?
O1 Mo1 O3 103.29(17) . . ?
O7 Mo1 O13 104.83(18) . . ?
O1 Mo1 O13 94.01(16) . . ?
O3 Mo1 O13 148.88(15) . . ?
O7 Mo1 O10 89.35(16) . 2_756 ?
O1 Mo1 O10 162.22(15) . 2_756 ?
O3 Mo1 O10 84.91(13) . 2_756 ?
O13 Mo1 O10 72.14(13) . 2_756 ?
O7 Mo1 O4 156.48(15) . . ?
O1 Mo1 O4 96.60(15) . . ?
O3 Mo1 O4 70.90(13) . . ?
O13 Mo1 O4 81.67(14) . . ?
O10 Mo1 O4 70.89(11) 2_756 . ?
O10 Cr1 O10 179.999(1) 2_756 . ?
O10 Cr1 O5 96.37(14) 2_756 . ?
O10 Cr1 O5 83.63(14) . . ?
O10 Cr1 O5 83.63(14) 2_756 2_756 ?
O10 Cr1 O5 96.37(14) . 2_756 ?
O5 Cr1 O5 179.999(1) . 2_756 ?
O10 Cr1 O4 84.54(13) 2_756 . ?
O10 Cr1 O4 95.46(13) . . ?
O5 Cr1 O4 83.02(13) . . ?
O5 Cr1 O4 96.98(13) 2_756 . ?
O10 Cr1 O4 95.46(13) 2_756 2_756 ?
O10 Cr1 O4 84.54(13) . 2_756 ?
O5 Cr1 O4 96.98(13) . 2_756 ?
O5 Cr1 O4 83.02(13) 2_756 2_756 ?
O4 Cr1 O4 179.999(1) . 2_756 ?
C4 N1 C5 103.0(4) . . ?
C4 N1 Mn4 145.6(4) . . ?
C5 N1 Mn4 110.9(3) . . ?
Mo1 O1 Mn4 146.7(2) . . ?
Mo3 O2 Mn4 144.3(2) 2_656 . ?
O6 Mo2 O12 104.7(2) . . ?
O6 Mo2 O9 103.26(18) . . ?
O12 Mo2 O9 93.96(17) . . ?
O6 Mo2 O3 94.87(17) . . ?
O12 Mo2 O3 100.05(17) . . ?
O9 Mo2 O3 153.45(15) . . ?
O6 Mo2 O5 93.51(17) . . ?
O12 Mo2 O5 160.21(16) . . ?
O9 Mo2 O5 74.12(13) . . ?
O3 Mo2 O5 85.70(14) . . ?
O6 Mo2 O4 159.37(16) . . ?
O12 Mo2 O4 92.59(16) . . ?
O9 Mo2 O4 86.31(13) . . ?
O3 Mo2 O4 70.74(13) . . ?
O5 Mo2 O4 71.29(12) . . ?
C3 C2 C8 120.1(6) . . ?
O11 Mo3 O2 105.8(2) . 2_656 ?
O11 Mo3 O9 101.15(18) . . ?
O2 Mo3 O9 95.04(17) 2_656 . ?
O11 Mo3 O13 97.21(18) . 2_756 ?
O2 Mo3 O13 97.74(17) 2_656 2_756 ?
O9 Mo3 O13 153.82(15) . 2_756 ?
O11 Mo3 O5 94.00(17) . . ?
O2 Mo3 O5 159.18(15) 2_656 . ?
O9 Mo3 O5 74.60(13) . . ?
O13 Mo3 O5 85.70(14) 2_756 . ?
O11 Mo3 O10 161.28(17) . . ?
O2 Mo3 O10 90.32(15) 2_656 . ?
O9 Mo3 O10 86.44(13) . . ?
O13 Mo3 O10 70.78(13) 2_756 . ?
O5 Mo3 O10 71.34(12) . . ?
C5 N3 N8 105.7(4) . . ?
Mo1 O3 Mo2 121.72(17) . . ?
N5 C3 C2 120.7(6) . . ?
N8 C4 N1 112.1(5) . . ?
O3W Mn4 O2W 94.73(19) . . ?
O3W Mn4 O2 90.38(18) . . ?
O2W Mn4 O2 174.67(17) . . ?
O3W Mn4 O1 85.70(15) . . ?
O2W Mn4 O1 96.41(17) . . ?
O2 Mn4 O1 82.44(15) . . ?
O3W Mn4 N4 169.91(16) . . ?
O2W Mn4 N4 87.89(16) . . ?
O2 Mn4 N4 87.33(15) . . ?
O1 Mn4 N4 103.72(15) . . ?
O3W Mn4 N1 93.58(16) . . ?
O2W Mn4 N1 92.34(18) . . ?
O2 Mn4 N1 88.84(16) . . ?
O1 Mn4 N1 171.25(17) . . ?
N4 Mn4 N1 76.56(16) . . ?
C9 N4 C7 101.7(4) . . ?
C9 N4 Mn4 146.6(3) . . ?
C7 N4 Mn4 110.8(3) . . ?
Cr1 O4 Mo2 100.55(13) . . ?
Cr1 O4 Mo1 100.39(13) . . ?
Mo2 O4 Mo1 94.16(12) . . ?
Cr1 O5 Mo3 104.51(14) . . ?
Cr1 O5 Mo2 105.12(14) . . ?
Mo3 O5 Mo2 94.36(13) . . ?
C3 N5 C10 121.2(5) . . ?
N3 C5 N1 112.4(5) . . ?
N3 C5 C7 127.8(5) . . ?
N1 C5 C7 119.6(4) . . ?
C9 N6 N7 105.9(4) . . ?
C10 C6 C8 119.8(5) . . ?
C7 N7 N6 105.9(4) . . ?
N7 C7 N4 113.0(5) . . ?
N7 C7 C5 126.4(4) . . ?
N4 C7 C5 120.5(5) . . ?
C4 N8 N3 106.8(4) . . ?
C6 C8 C2 117.8(5) . . ?
C6 C8 C9 121.8(5) . . ?
C2 C8 C9 120.3(5) . . ?
Mo3 O9 Mo2 112.76(16) . . ?
N6 C9 N4 113.4(5) . . ?
N6 C9 C8 122.0(5) . . ?
N4 C9 C8 124.5(5) . . ?
Cr1 O10 Mo1 104.18(14) . 2_756 ?
Cr1 O10 Mo3 100.49(14) . . ?
Mo1 O10 Mo3 93.45(12) 2_756 . ?
N5 C10 C6 120.4(6) . . ?
Mo1 O13 Mo3 118.79(17) . 2_756 ?

_diffrn_measured_fraction_theta_max 0.963
_diffrn_reflns_theta_full        28.38
_diffrn_measured_fraction_theta_full 0.963
_refine_diff_density_max         1.809
_refine_diff_density_min         -1.022
_refine_diff_density_rms         0.179
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_complex2
_database_code_depnum_ccdc_archive 'CCDC 1514242'
_audit_update_record             
;
2016-12-27 deposited with the CCDC.
2017-04-28 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C14 H23 Cr Mn Mo6 N4 O27'
_chemical_formula_weight         1361.94

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cr Cr 0.3209 0.6236 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Triclinic
_symmetry_space_group_name_H-M   'P -1'

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   7.0352(16)
_cell_length_b                   11.367(3)
_cell_length_c                   21.063(5)
_cell_angle_alpha                88.386(4)
_cell_angle_beta                 89.989(5)
_cell_angle_gamma                77.187(4)
_cell_volume                     1641.7(6)
_cell_formula_units_Z            2
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    3662
_cell_measurement_theta_min      2.6302
_cell_measurement_theta_max      28.2821

_exptl_crystal_description       BLOCK
_exptl_crystal_colour            YELLOW
_exptl_crystal_size_max          0.32
_exptl_crystal_size_mid          0.24
_exptl_crystal_size_min          0.19
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    2.755
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1292
_exptl_absorpt_coefficient_mu    3.012
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.424
_exptl_absorpt_correction_T_max  0.564
_exptl_absorpt_process_details   SADABS

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            12115
_diffrn_reflns_av_R_equivalents  0.0403
_diffrn_reflns_av_sigmaI/netI    0.0790
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_theta_min         0.97
_diffrn_reflns_theta_max         28.44
_reflns_number_total             8273
_reflns_number_gt                6719
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'SMART (Bruker, 2001)'
_computing_cell_refinement       'SMART (Bruker, 2001)'
_computing_data_reduction        'SAINT+ (Bruker, 1999)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_molecular_graphics    'PLATON (Spek, 2003)'
_computing_publication_material  'SHELXTL (1998)'

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0001P)²+180.6374P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         8110
_refine_ls_number_parameters     500
_refine_ls_number_restraints     24
_refine_ls_R_factor_all          0.1056
_refine_ls_R_factor_gt           0.0928
_refine_ls_wR_factor_ref         0.2389
_refine_ls_wR_factor_gt          0.2328
_refine_ls_goodness_of_fit_ref   1.071
_refine_ls_restrained_S_all      1.070
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.58700(18) 1.21201(11) 0.48466(6) 0.0116(3) Uani 0.9665(15) 1 d P A 1
Mo1' Mo 0.539(5) 1.324(3) 0.4885(17) 0.0116(3) Uani 0.0335(15) 1 d P A 2
Mn1 Mn 0.5179(3) 0.8548(2) 0.25282(10) 0.0132(4) Uani 1 1 d . . .
Cr1 Cr 1.0000 1.0000 0.5000 0.0081(6) Uani 1 2 d S . .
O1 O 0.6556(18) 0.9497(12) 0.3186(6) 0.026(3) Uani 1 1 d . . .
O1W O 0.2735(17) 1.0203(10) 0.2472(6) 0.022(2) Uani 1 1 d . . .
H1WA H 0.2033 1.0182 0.2799 0.026 Uiso 1 1 d R A .
H1WB H 0.1998 1.0269 0.2147 0.026 Uiso 1 1 d R . .
N1 N 0.656(2) 0.6551(13) 0.2490(7) 0.020(3) Uani 1 1 d . . .
Mo2 Mo 0.75980(19) 1.04597(12) 0.36195(6) 0.0122(3) Uani 0.9665(15) 1 d P A 1
Mo2' Mo 0.785(5) 0.938(3) 0.3607(17) 0.0122(3) Uani 0.0335(15) 1 d P A 2
Cr2 Cr 1.0000 1.0000 0.0000 0.0082(6) Uani 1 2 d S . .
O2 O 0.6619(19) 0.9230(12) 0.1757(5) 0.025(3) Uani 1 1 d . . .
N2 N 0.832(3) 0.5151(15) 0.0691(8) 0.035(4) Uani 1 1 d . . .
H2A H 0.7641 0.5869 0.0743 0.042 Uiso 1 1 calc R . .
C2 C 0.784(3) 0.4873(16) 0.1826(9) 0.027(4) Uani 1 1 d . . .
Mo3 Mo 0.75709(19) 1.03070(12) 0.13606(6) 0.0126(3) Uani 0.9665(15) 1 d P A 1
Mo3' Mo 0.725(5) 1.143(4) 0.1382(18) 0.0126(3) Uani 0.0335(15) 1 d P A 2
N3 N 0.264(3) 0.4721(16) 0.2214(10) 0.045(5) Uani 1 1 d . . .
H3B H 0.2566 0.5331 0.1957 0.054 Uiso 1 1 calc R . .
C3 C 0.290(4) 0.2757(17) 0.3012(10) 0.044(6) Uani 1 1 d . . .
H3A H 0.3035 0.2079 0.3280 0.052 Uiso 1 1 calc R . .
Mo4 Mo 0.15979(19) 0.81766(12) 0.12267(6) 0.0120(3) Uani 0.9665(15) 1 d P . 1
Mo4' Mo 0.193(5) 0.720(3) 0.1186(17) 0.0120(3) Uani 0.0335(15) 1 d P A 2
O4 O 1.3607(17) 0.8085(10) 0.3332(6) 0.022(2) Uani 1 1 d . . .
C4 C 0.904(3) 0.4834(19) 0.0082(10) 0.033(4) Uani 1 1 d U . .
H4A H 0.8067 0.5224 -0.0229 0.039 Uiso 1 1 calc R . .
H4B H 0.9199 0.3969 0.0044 0.039 Uiso 1 1 calc R . .
N4 N 0.035(3) 0.4986(14) 0.4119(8) 0.031(4) Uani 1 1 d . . .
H4D H 0.0520 0.5625 0.3919 0.037 Uiso 1 1 calc R . .
Mo5 Mo 0.58044(18) 1.20869(12) 0.01249(6) 0.0124(3) Uani 0.9665(15) 1 d P . 1
Mo5' Mo 0.547(5) 1.310(3) 0.0205(19) 0.0124(3) Uani 0.0335(15) 1 d P . 2
Mo6 Mo 1.15435(19) 0.82368(11) 0.37986(6) 0.0113(3) Uani 0.9665(15) 1 d P . 1
Mo6' Mo 1.195(5) 0.718(3) 0.3776(17) 0.0113(3) Uani 0.0335(15) 1 d P . 2
C6 C 0.201(2) 0.3898(15) 0.3220(8) 0.022(3) Uani 1 1 d . . .
O10 O 0.3599(17) 0.8067(11) 0.1711(6) 0.024(3) Uani 1 1 d . . .
O11 O 0.5412(18) 1.3281(11) 0.0614(6) 0.024(3) Uani 1 1 d . . .
O13 O 0.7261(19) 1.1755(12) 0.3183(6) 0.029(3) Uani 1 1 d . . .
O14 O 1.0309(16) 0.9813(9) 0.3423(5) 0.014(2) Uani 1 1 d . . .
O15 O 1.0263(15) 0.9727(10) 0.1575(5) 0.016(2) Uani 1 1 d . . .
O16 O 0.7057(19) 1.1553(11) 0.1798(6) 0.027(3) Uani 1 1 d . . .
O17 O 0.5551(16) 1.0787(11) 0.0700(5) 0.019(2) Uani 1 1 d . . .
O18 O 0.3647(18) 1.2238(12) -0.0287(6) 0.026(3) Uani 1 1 d . . .
O19 O 0.8805(16) 1.1327(9) 0.0568(5) 0.014(2) Uani 1 1 d . . .
O20 O 0.2503(14) 0.9498(9) 0.0467(5) 0.0108(19) Uani 1 1 d . . .
O21 O 0.9019(14) 0.8947(9) 0.0611(5) 0.012(2) Uani 1 1 d . . .
O22 O 0.966(2) 0.3343(14) 0.1172(7) 0.040(3) Uani 1 1 d . . .
O23 O 0.097(2) 0.2920(12) 0.4129(7) 0.032(3) Uani 1 1 d U . .
O24 O 0.2677(18) 0.7282(11) 0.0508(5) 0.022(2) Uani 1 1 d . . .
O25 O 0.0366(19) 0.7200(13) 0.1556(6) 0.032(3) Uani 1 1 d . . .
C25 C 0.195(3) 0.4865(16) 0.2806(9) 0.033(4) Uani 1 1 d . . .
H25A H 0.1416 0.5639 0.2942 0.039 Uiso 1 1 calc R . .
O26 O 0.8956(15) 0.9028(9) 0.4387(5) 0.014(2) Uani 1 1 d . . .
O27 O 0.5554(16) 1.0899(10) 0.4253(5) 0.017(2) Uani 1 1 d . . .
O28 O 0.8849(15) 1.1350(9) 0.4423(5) 0.013(2) Uani 1 1 d U . .
O29 O 0.5439(19) 1.3370(11) 0.4362(6) 0.025(3) Uani 1 1 d . . .
O30 O 0.3766(16) 1.2181(10) 0.5269(6) 0.021(2) Uani 1 1 d . . .
O31 O 0.7489(17) 1.2697(10) 0.5473(5) 0.017(2) Uani 1 1 d . . .
O32 O 0.7514(15) 1.0496(10) 0.5461(5) 0.013(2) Uani 1 1 d . . .
O33 O 1.022(2) 0.7307(11) 0.3471(6) 0.028(3) Uani 1 1 d . . .
C40 C -0.073(3) 0.5093(19) 0.4726(10) 0.036(5) Uani 1 1 d . . .
H40A H -0.1516 0.4490 0.4755 0.044 Uiso 1 1 calc R . .
H40B H -0.1598 0.5885 0.4746 0.044 Uiso 1 1 calc R . .
C43 C 0.715(3) 0.6121(15) 0.1926(8) 0.023(3) Uani 1 1 d . A .
H43A H 0.7112 0.6661 0.1583 0.028 Uiso 1 1 calc R . .
C44 C 0.352(3) 0.2671(19) 0.2438(10) 0.034(4) Uani 1 1 d U . .
H44A H 0.4067 0.1900 0.2300 0.040 Uiso 1 1 calc R . .
C45 C 0.783(3) 0.4111(15) 0.2344(10) 0.029(4) Uani 1 1 d . A .
H45A H 0.8273 0.3284 0.2297 0.035 Uiso 1 1 calc R . .
C46 C 0.106(3) 0.3903(15) 0.3881(7) 0.020(3) Uani 1 1 d . . .
C48 C 0.346(3) 0.357(2) 0.2028(10) 0.040(5) Uani 1 1 d . . .
H48A H 0.3961 0.3434 0.1622 0.048 Uiso 1 1 calc R . .
C49 C 0.722(3) 0.4524(16) 0.2913(10) 0.029(4) Uani 1 1 d . . .
H49A H 0.7170 0.3998 0.3256 0.035 Uiso 1 1 calc R A .
C50 C 0.664(3) 0.5782(16) 0.2975(8) 0.025(4) Uani 1 1 d . A .
H50A H 0.6288 0.6084 0.3374 0.030 Uiso 1 1 calc R . .
C51 C 0.866(3) 0.4389(17) 0.1193(9) 0.030(4) Uani 1 1 d . A .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O29 1.697(12) . ?
Mo1 O30 1.716(11) . ?
Mo1 O27 1.943(11) . ?
Mo1 O31 1.962(11) . ?
Mo1 O28 2.277(10) . ?
Mo1 O32 2.311(11) . ?
Mo1' O29 1.11(4) . ?
Mo1' O31 1.91(4) . ?
Mo1' O30 1.99(4) . ?
Mn1 O2 2.131(12) . ?
Mn1 O1 2.138(11) . ?
Mn1 O4 2.138(12) 1_455 ?
Mn1 O10 2.195(12) . ?
Mn1 O1W 2.250(12) . ?
Mn1 N1 2.266(14) . ?
Cr1 O28 1.957(10) 2_776 ?
Cr1 O28 1.957(10) . ?
Cr1 O26 1.966(10) . ?
Cr1 O26 1.966(10) 2_776 ?
Cr1 O32 1.978(10) 2_776 ?
Cr1 O32 1.978(10) . ?
O1 Mo2' 1.26(4) . ?
O1 Mo2 1.727(12) . ?
O1W H1WA 0.8500 . ?
O1W H1WB 0.8499 . ?
N1 C50 1.32(2) . ?
N1 C43 1.33(2) . ?
Mo2 O13 1.685(13) . ?
Mo2 O14 1.935(11) . ?
Mo2 O27 1.953(11) . ?
Mo2 O28 2.271(10) . ?
Mo2 O26 2.310(11) . ?
Mo2' O26 1.81(4) . ?
Mo2' O14 1.93(4) . ?
Mo2' O27 2.52(4) . ?
Cr2 O21 1.961(10) . ?
Cr2 O21 1.961(10) 2_775 ?
Cr2 O20 1.979(10) 1_655 ?
Cr2 O20 1.979(10) 2_675 ?
Cr2 O19 1.988(11) 2_775 ?
Cr2 O19 1.988(11) . ?
O2 Mo3 1.718(12) . ?
N2 C51 1.33(2) . ?
N2 C4 1.41(3) . ?
N2 H2A 0.8600 . ?
C2 C45 1.37(3) . ?
C2 C43 1.42(2) . ?
C2 C51 1.52(3) . ?
Mo3 O16 1.683(11) . ?
Mo3 O15 1.912(11) . ?
Mo3 O17 1.967(11) . ?
Mo3 O19 2.286(10) . ?
Mo3 O21 2.315(11) . ?
Mo3' O16 0.90(4) . ?
Mo3' O19 2.03(4) . ?
Mo3' O17 2.11(4) . ?
Mo3' Mo5' 3.16(5) . ?
N3 C25 1.34(3) . ?
N3 C48 1.37(3) . ?
N3 H3B 0.8600 . ?
C3 C44 1.29(3) . ?
C3 C6 1.39(2) . ?
C3 H3A 0.9300 . ?
Mo4 O25 1.687(13) . ?
Mo4 O10 1.719(11) . ?
Mo4 O24 1.909(12) . ?
Mo4 O15 1.965(11) 1_455 ?
Mo4 O21 2.230(10) 1_455 ?
Mo4 O20 2.348(10) . ?
Mo4' O25 1.35(4) . ?
Mo4' O24 1.53(4) . ?
Mo4' O10 2.03(4) . ?
O4 Mo6 1.732(11) . ?
O4 Mo6' 1.94(4) . ?
O4 Mn1 2.138(11) 1_655 ?
C4 C4 1.52(4) 2_765 ?
C4 H4A 0.9700 . ?
C4 H4B 0.9700 . ?
N4 C46 1.33(2) . ?
N4 C40 1.48(3) . ?
N4 H4D 0.8600 . ?
Mo5 O11 1.701(12) . ?
Mo5 O18 1.721(12) . ?
Mo5 O17 1.923(11) . ?
Mo5 O24 1.929(12) 2_675 ?
Mo5 O19 2.284(11) . ?
Mo5 O20 2.322(10) 2_675 ?
Mo5' O11 0.89(4) . ?
Mo5' O24 1.98(4) 2_675 ?
Mo5' O18 2.07(4) . ?
Mo6 O33 1.713(13) . ?
Mo6 O31 1.879(11) 2_776 ?
Mo6 O14 1.955(11) . ?
Mo6 O26 2.234(10) . ?
Mo6 O32 2.345(10) 2_776 ?
Mo6' O33 1.35(4) . ?
Mo6' O31 1.65(4) 2_776 ?
C6 C25 1.38(2) . ?
C6 C46 1.54(2) . ?
O15 Mo4 1.965(11) 1_655 ?
O20 Cr2 1.979(10) 1_455 ?
O20 Mo5 2.322(10) 2_675 ?
O21 Mo4 2.230(10) 1_655 ?
O22 C51 1.24(2) . ?
O23 C46 1.23(2) . ?
O24 Mo5 1.929(12) 2_675 ?
O24 Mo5' 1.98(4) 2_675 ?
C25 H25A 0.9300 . ?
O31 Mo6' 1.65(4) 2_776 ?
O31 Mo6 1.879(11) 2_776 ?
O32 Mo6 2.345(10) 2_776 ?
C40 C40 1.53(4) 2_566 ?
C40 H40A 0.9700 . ?
C40 H40B 0.9700 . ?
C43 H43A 0.9300 . ?
C44 C48 1.31(3) . ?
C44 H44A 0.9300 . ?
C45 C49 1.34(3) . ?
C45 H45A 0.9300 . ?
C48 H48A 0.9300 . ?
C49 C50 1.41(2) . ?
C49 H49A 0.9300 . ?
C50 H50A 0.9300 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O29 Mo1 O30 105.9(6) . . ?
O29 Mo1 O27 100.8(5) . . ?
O30 Mo1 O27 98.0(5) . . ?
O29 Mo1 O31 97.1(5) . . ?
O30 Mo1 O31 101.0(5) . . ?
O27 Mo1 O31 149.1(5) . . ?
O29 Mo1 O28 93.9(5) . . ?
O30 Mo1 O28 159.5(5) . . ?
O27 Mo1 O28 72.5(4) . . ?
O31 Mo1 O28 81.3(4) . . ?
O29 Mo1 O32 160.7(5) . . ?
O30 Mo1 O32 91.6(5) . . ?
O27 Mo1 O32 84.4(4) . . ?
O31 Mo1 O32 71.0(4) . . ?
O28 Mo1 O32 69.8(4) . . ?
O29 Mo1' O31 129(3) . . ?
O29 Mo1' O30 120(3) . . ?
O31 Mo1' O30 93.5(16) . . ?
O2 Mn1 O1 90.6(5) . . ?
O2 Mn1 O4 173.1(5) . 1_455 ?
O1 Mn1 O4 85.5(5) . 1_455 ?
O2 Mn1 O10 78.7(5) . . ?
O1 Mn1 O10 163.9(5) . . ?
O4 Mn1 O10 104.0(5) 1_455 . ?
O2 Mn1 O1W 90.6(5) . . ?
O1 Mn1 O1W 86.9(5) . . ?
O4 Mn1 O1W 83.5(4) 1_455 . ?
O10 Mn1 O1W 81.4(4) . . ?
O2 Mn1 N1 100.5(5) . . ?
O1 Mn1 N1 113.9(5) . . ?
O4 Mn1 N1 86.2(5) 1_455 . ?
O10 Mn1 N1 80.2(5) . . ?
O1W Mn1 N1 156.0(5) . . ?
O28 Cr1 O28 180.0(5) 2_776 . ?
O28 Cr1 O26 95.9(4) 2_776 . ?
O28 Cr1 O26 84.1(4) . . ?
O28 Cr1 O26 84.1(4) 2_776 2_776 ?
O28 Cr1 O26 95.9(4) . 2_776 ?
O26 Cr1 O26 180.0(5) . 2_776 ?
O28 Cr1 O32 83.6(4) 2_776 2_776 ?
O28 Cr1 O32 96.4(4) . 2_776 ?
O26 Cr1 O32 85.5(4) . 2_776 ?
O26 Cr1 O32 94.5(4) 2_776 2_776 ?
O28 Cr1 O32 96.4(4) 2_776 . ?
O28 Cr1 O32 83.6(4) . . ?
O26 Cr1 O32 94.5(4) . . ?
O26 Cr1 O32 85.5(4) 2_776 . ?
O32 Cr1 O32 179.999(3) 2_776 . ?
Mo2' O1 Mo2 43.9(18) . . ?
Mo2' O1 Mn1 145(2) . . ?
Mo2 O1 Mn1 170.1(8) . . ?
Mn1 O1W H1WA 107.1 . . ?
Mn1 O1W H1WB 115.8 . . ?
H1WA O1W H1WB 107.7 . . ?
C50 N1 C43 118.4(15) . . ?
C50 N1 Mn1 124.1(11) . . ?
C43 N1 Mn1 117.1(11) . . ?
O13 Mo2 O1 105.8(6) . . ?
O13 Mo2 O14 98.6(5) . . ?
O1 Mo2 O14 99.1(5) . . ?
O13 Mo2 O27 100.6(6) . . ?
O1 Mo2 O27 98.4(5) . . ?
O14 Mo2 O27 149.3(4) . . ?
O13 Mo2 O28 89.9(5) . . ?
O1 Mo2 O28 163.2(5) . . ?
O14 Mo2 O28 83.8(4) . . ?
O27 Mo2 O28 72.5(4) . . ?
O13 Mo2 O26 157.7(5) . . ?
O1 Mo2 O26 95.3(5) . . ?
O14 Mo2 O26 70.5(4) . . ?
O27 Mo2 O26 82.9(4) . . ?
O28 Mo2 O26 70.0(4) . . ?
O1 Mo2' O26 157(3) . . ?
O1 Mo2' O14 121(2) . . ?
O26 Mo2' O14 82.4(15) . . ?
O1 Mo2' O27 89(2) . . ?
O26 Mo2' O27 80.0(13) . . ?
O14 Mo2' O27 114.2(17) . . ?
O21 Cr2 O21 180.0(5) . 2_775 ?
O21 Cr2 O20 85.6(4) . 1_655 ?
O21 Cr2 O20 94.4(4) 2_775 1_655 ?
O21 Cr2 O20 94.4(4) . 2_675 ?
O21 Cr2 O20 85.6(4) 2_775 2_675 ?
O20 Cr2 O20 179.999(1) 1_655 2_675 ?
O21 Cr2 O19 94.7(4) . 2_775 ?
O21 Cr2 O19 85.3(4) 2_775 2_775 ?
O20 Cr2 O19 83.5(4) 1_655 2_775 ?
O20 Cr2 O19 96.5(4) 2_675 2_775 ?
O21 Cr2 O19 85.3(4) . . ?
O21 Cr2 O19 94.7(4) 2_775 . ?
O20 Cr2 O19 96.5(4) 1_655 . ?
O20 Cr2 O19 83.5(4) 2_675 . ?
O19 Cr2 O19 179.999(3) 2_775 . ?
Mo3 O2 Mn1 154.3(7) . . ?
C51 N2 C4 123.0(18) . . ?
C51 N2 H2A 118.5 . . ?
C4 N2 H2A 118.5 . . ?
C45 C2 C43 116.5(17) . . ?
C45 C2 C51 120.9(17) . . ?
C43 C2 C51 122.5(16) . . ?
O16 Mo3 O2 106.7(6) . . ?
O16 Mo3 O15 99.9(6) . . ?
O2 Mo3 O15 99.3(6) . . ?
O16 Mo3 O17 99.2(6) . . ?
O2 Mo3 O17 98.7(5) . . ?
O15 Mo3 O17 148.6(5) . . ?
O16 Mo3 O19 91.0(5) . . ?
O2 Mo3 O19 161.3(5) . . ?
O15 Mo3 O19 83.0(4) . . ?
O17 Mo3 O19 72.0(4) . . ?
O16 Mo3 O21 160.5(5) . . ?
O2 Mo3 O21 92.0(5) . . ?
O15 Mo3 O21 70.9(4) . . ?
O17 Mo3 O21 83.0(4) . . ?
O19 Mo3 O21 71.1(4) . . ?
O16 Mo3' O19 154(3) . . ?
O16 Mo3' O17 131(3) . . ?
O19 Mo3' O17 74.7(14) . . ?
O16 Mo3' Mo5' 129(3) . . ?
O19 Mo3' Mo5' 61.4(12) . . ?
O17 Mo3' Mo5' 60.0(12) . . ?
C25 N3 C48 118.1(18) . . ?
C25 N3 H3B 120.9 . . ?
C48 N3 H3B 120.9 . . ?
C44 C3 C6 118(2) . . ?
C44 C3 H3A 121.1 . . ?
C6 C3 H3A 121.1 . . ?
O25 Mo4 O10 104.6(6) . . ?
O25 Mo4 O24 99.7(6) . . ?
O10 Mo4 O24 102.5(5) . . ?
O25 Mo4 O15 102.7(6) . 1_455 ?
O10 Mo4 O15 92.9(5) . 1_455 ?
O24 Mo4 O15 148.6(5) . 1_455 ?
O25 Mo4 O21 89.5(5) . 1_455 ?
O10 Mo4 O21 161.5(5) . 1_455 ?
O24 Mo4 O21 86.6(4) . 1_455 ?
O15 Mo4 O21 71.9(4) 1_455 1_455 ?
O25 Mo4 O20 158.9(5) . . ?
O10 Mo4 O20 96.0(5) . . ?
O24 Mo4 O20 70.9(4) . . ?
O15 Mo4 O20 80.5(4) 1_455 . ?
O21 Mo4 O20 71.5(3) 1_455 . ?
O25 Mo4' O24 146(3) . . ?
O25 Mo4' O10 104(2) . . ?
O24 Mo4' O10 104(2) . . ?
Mo6 O4 Mo6' 36.6(11) . . ?
Mo6 O4 Mn1 152.9(7) . 1_655 ?
Mo6' O4 Mn1 154.3(12) . 1_655 ?
N2 C4 C4 115(2) . 2_765 ?
N2 C4 H4A 108.5 . . ?
C4 C4 H4A 108.5 2_765 . ?
N2 C4 H4B 108.5 . . ?
C4 C4 H4B 108.5 2_765 . ?
H4A C4 H4B 107.5 . . ?
C46 N4 C40 120.2(15) . . ?
C46 N4 H4D 119.9 . . ?
C40 N4 H4D 119.9 . . ?
O11 Mo5 O18 104.6(6) . . ?
O11 Mo5 O17 101.8(5) . . ?
O18 Mo5 O17 98.7(5) . . ?
O11 Mo5 O24 97.8(6) . 2_675 ?
O18 Mo5 O24 99.8(5) . 2_675 ?
O17 Mo5 O24 148.6(5) . 2_675 ?
O11 Mo5 O19 91.4(5) . . ?
O18 Mo5 O19 163.3(5) . . ?
O17 Mo5 O19 72.7(4) . . ?
O24 Mo5 O19 82.5(4) 2_675 . ?
O11 Mo5 O20 159.1(5) . 2_675 ?
O18 Mo5 O20 95.0(5) . 2_675 ?
O17 Mo5 O20 82.1(4) . 2_675 ?
O24 Mo5 O20 71.2(4) 2_675 2_675 ?
O19 Mo5 O20 70.0(4) . 2_675 ?
O11 Mo5' O24 142(3) . 2_675 ?
O11 Mo5' O18 127(3) . . ?
O24 Mo5' O18 87.1(16) 2_675 . ?
O11 Mo5' Mo3' 52(2) . . ?
O24 Mo5' Mo3' 107.6(16) 2_675 . ?
O18 Mo5' Mo3' 108.3(16) . . ?
O33 Mo6 O4 104.8(6) . . ?
O33 Mo6 O31 99.6(5) . 2_776 ?
O4 Mo6 O31 102.1(5) . 2_776 ?
O33 Mo6 O14 102.4(5) . . ?
O4 Mo6 O14 93.9(5) . . ?
O31 Mo6 O14 148.5(4) 2_776 . ?
O33 Mo6 O26 88.9(5) . . ?
O4 Mo6 O26 162.2(5) . . ?
O31 Mo6 O26 86.3(4) 2_776 . ?
O14 Mo6 O26 71.9(4) . . ?
O33 Mo6 O32 158.7(5) . 2_776 ?
O4 Mo6 O32 96.1(5) . 2_776 ?
O31 Mo6 O32 71.6(4) 2_776 2_776 ?
O14 Mo6 O32 79.9(4) . 2_776 ?
O26 Mo6 O32 71.5(4) . 2_776 ?
O33 Mo6' O31 132(3) . 2_776 ?
O33 Mo6' O4 111(2) . . ?
O31 Mo6' O4 102.9(19) 2_776 . ?
C25 C6 C3 117.5(18) . . ?
C25 C6 C46 127.7(16) . . ?
C3 C6 C46 114.6(17) . . ?
Mo4 O10 Mo4' 32.3(11) . . ?
Mo4 O10 Mn1 154.4(7) . . ?
Mo4' O10 Mn1 159.9(12) . . ?
Mo5' O11 Mo5 38(3) . . ?
Mo2' O14 Mo2 36.1(11) . . ?
Mo2' O14 Mo6 86.3(12) . . ?
Mo2 O14 Mo6 117.6(5) . . ?
Mo3 O15 Mo4 117.3(5) . 1_655 ?
Mo3' O16 Mo3 46(3) . . ?
Mo5 O17 Mo3 117.0(6) . . ?
Mo5 O17 Mo3' 89.9(11) . . ?
Mo3 O17 Mo3' 35.3(11) . . ?
Mo5 O18 Mo5' 33.3(11) . . ?
Cr2 O19 Mo3' 134.7(12) . . ?
Cr2 O19 Mo5 103.8(4) . . ?
Mo3' O19 Mo5 82.7(11) . . ?
Cr2 O19 Mo3 101.9(4) . . ?
Mo3' O19 Mo3 32.9(11) . . ?
Mo5 O19 Mo3 93.1(4) . . ?
Cr2 O20 Mo5 102.8(4) 1_455 2_675 ?
Cr2 O20 Mo4 99.1(4) 1_455 . ?
Mo5 O20 Mo4 92.3(4) 2_675 . ?
Cr2 O21 Mo4 103.8(4) . 1_655 ?
Cr2 O21 Mo3 101.7(4) . . ?
Mo4 O21 Mo3 93.5(4) 1_655 . ?
Mo4' O24 Mo4 34.7(15) . . ?
Mo4' O24 Mo5 151.9(16) . 2_675 ?
Mo4 O24 Mo5 122.6(6) . 2_675 ?
Mo4' O24 Mo5' 156.5(19) . 2_675 ?
Mo4 O24 Mo5' 153.9(13) . 2_675 ?
Mo5 O24 Mo5' 33.8(11) 2_675 2_675 ?
Mo4' O25 Mo4 40.0(17) . . ?
N3 C25 C6 121.9(18) . . ?
N3 C25 H25A 119.1 . . ?
C6 C25 H25A 119.1 . . ?
Mo2' O26 Cr1 132.5(13) . . ?
Mo2' O26 Mo6 81.4(12) . . ?
Cr1 O26 Mo6 103.5(4) . . ?
Mo2' O26 Mo2 30.9(12) . . ?
Cr1 O26 Mo2 102.1(4) . . ?
Mo6 O26 Mo2 94.1(4) . . ?
Mo1 O27 Mo2 116.5(5) . . ?
Mo1 O27 Mo2' 134.6(10) . . ?
Mo2 O27 Mo2' 27.6(9) . . ?
Cr1 O28 Mo2 103.8(4) . . ?
Cr1 O28 Mo1 104.2(4) . . ?
Mo2 O28 Mo1 93.5(4) . . ?
Mo1' O29 Mo1 47(2) . . ?
Mo1 O30 Mo1' 38.4(11) . . ?
Mo6' O31 Mo6 38.0(13) 2_776 2_776 ?
Mo6' O31 Mo1' 140.5(18) 2_776 . ?
Mo6 O31 Mo1' 148.4(13) 2_776 . ?
Mo6' O31 Mo1 148.4(14) 2_776 . ?
Mo6 O31 Mo1 121.5(6) 2_776 . ?
Mo1' O31 Mo1 37.5(11) . . ?
Cr1 O32 Mo1 102.4(4) . . ?
Cr1 O32 Mo6 99.4(4) . 2_776 ?
Mo1 O32 Mo6 92.1(4) . 2_776 ?
Mo6' O33 Mo6 42.9(16) . . ?
N4 C40 C40 109(2) . 2_566 ?
N4 C40 H40A 109.9 . . ?
C40 C40 H40A 109.9 2_566 . ?
N4 C40 H40B 109.9 . . ?
C40 C40 H40B 109.9 2_566 . ?
H40A C40 H40B 108.3 . . ?
N1 C43 C2 122.5(16) . . ?
N1 C43 H43A 118.7 . . ?
C2 C43 H43A 118.7 . . ?
C3 C44 C48 126(2) . . ?
C3 C44 H44A 117.0 . . ?
C48 C44 H44A 117.0 . . ?
C49 C45 C2 121.9(17) . . ?
C49 C45 H45A 119.1 . . ?
C2 C45 H45A 119.1 . . ?
O23 C46 N4 126.4(16) . . ?
O23 C46 C6 117.6(15) . . ?
N4 C46 C6 116.0(14) . . ?
C44 C48 N3 119(2) . . ?
C44 C48 H48A 120.7 . . ?
N3 C48 H48A 120.7 . . ?
C45 C49 C50 117.7(17) . . ?
C45 C49 H49A 121.2 . . ?
C50 C49 H49A 121.2 . . ?
N1 C50 C49 122.8(16) . . ?
N1 C50 H50A 118.6 . . ?
C49 C50 H50A 118.6 . . ?
O22 C51 N2 123.4(18) . . ?
O22 C51 C2 119.5(17) . . ?
N2 C51 C2 117.0(17) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 Mn1 O1 Mo2' -106(3) . . . . ?
O4 Mn1 O1 Mo2' 79(3) 1_455 . . . ?
O10 Mn1 O1 Mo2' -154(3) . . . . ?
O1W Mn1 O1 Mo2' 163(3) . . . . ?
N1 Mn1 O1 Mo2' -5(3) . . . . ?
O2 Mn1 O1 Mo2 39(4) . . . . ?
O4 Mn1 O1 Mo2 -135(4) 1_455 . . . ?
O10 Mn1 O1 Mo2 -8(6) . . . . ?
O1W Mn1 O1 Mo2 -51(4) . . . . ?
N1 Mn1 O1 Mo2 141(4) . . . . ?
O2 Mn1 N1 C50 158.0(14) . . . . ?
O1 Mn1 N1 C50 62.6(15) . . . . ?
O4 Mn1 N1 C50 -20.7(15) 1_455 . . . ?
O10 Mn1 N1 C50 -125.6(15) . . . . ?
O1W Mn1 N1 C50 -85.5(18) . . . . ?
O2 Mn1 N1 C43 -29.2(13) . . . . ?
O1 Mn1 N1 C43 -124.5(12) . . . . ?
O4 Mn1 N1 C43 152.1(13) 1_455 . . . ?
O10 Mn1 N1 C43 47.2(13) . . . . ?
O1W Mn1 N1 C43 87.3(17) . . . . ?
Mo2' O1 Mo2 O13 156(2) . . . . ?
Mn1 O1 Mo2 O13 4(5) . . . . ?
Mo2' O1 Mo2 O14 54(2) . . . . ?
Mn1 O1 Mo2 O14 -98(4) . . . . ?
Mo2' O1 Mo2 O27 -100(2) . . . . ?
Mn1 O1 Mo2 O27 108(4) . . . . ?
Mo2' O1 Mo2 O28 -45(3) . . . . ?
Mn1 O1 Mo2 O28 163(3) . . . . ?
Mo2' O1 Mo2 O26 -17(2) . . . . ?
Mn1 O1 Mo2 O26 -169(4) . . . . ?
Mo2 O1 Mo2' O26 110(8) . . . . ?
Mn1 O1 Mo2' O26 -78(8) . . . . ?
Mo2 O1 Mo2' O14 -69(2) . . . . ?
Mn1 O1 Mo2' O14 103(3) . . . . ?
Mo2 O1 Mo2' O27 49.0(14) . . . . ?
Mn1 O1 Mo2' O27 -139(2) . . . . ?
O1 Mn1 O2 Mo3 -35.8(18) . . . . ?
O4 Mn1 O2 Mo3 19(5) 1_455 . . . ?
O10 Mn1 O2 Mo3 132.1(18) . . . . ?
O1W Mn1 O2 Mo3 51.0(18) . . . . ?
N1 Mn1 O2 Mo3 -150.3(17) . . . . ?
Mn1 O2 Mo3 O16 -3.6(19) . . . . ?
Mn1 O2 Mo3 O15 99.8(17) . . . . ?
Mn1 O2 Mo3 O17 -106.0(17) . . . . ?
Mn1 O2 Mo3 O19 -164.4(10) . . . . ?
Mn1 O2 Mo3 O21 170.8(17) . . . . ?
C51 N2 C4 C4 -95(3) . . . 2_765 ?
O16 Mo3' Mo5' O11 10(5) . . . . ?
O19 Mo3' Mo5' O11 -142(3) . . . . ?
O17 Mo3' Mo5' O11 130(3) . . . . ?
O16 Mo3' Mo5' O24 154(4) . . . 2_675 ?
O19 Mo3' Mo5' O24 2.1(16) . . . 2_675 ?
O17 Mo3' Mo5' O24 -86.1(17) . . . 2_675 ?
O16 Mo3' Mo5' O18 -113(4) . . . . ?
O19 Mo3' Mo5' O18 94.9(18) . . . . ?
O17 Mo3' Mo5' O18 6.8(15) . . . . ?
Mo6' O4 Mo6 O33 -46.6(19) . . . . ?
Mn1 O4 Mo6 O33 86.7(16) 1_655 . . . ?
Mo6' O4 Mo6 O31 56.9(19) . . . 2_776 ?
Mn1 O4 Mo6 O31 -169.8(15) 1_655 . . 2_776 ?
Mo6' O4 Mo6 O14 -150.5(19) . . . . ?
Mn1 O4 Mo6 O14 -17.1(16) 1_655 . . . ?
Mo6' O4 Mo6 O26 174(2) . . . . ?
Mn1 O4 Mo6 O26 -53(3) 1_655 . . . ?
Mo6' O4 Mo6 O32 129.3(19) . . . 2_776 ?
Mn1 O4 Mo6 O32 -97.4(16) 1_655 . . 2_776 ?
Mo6 O4 Mo6' O33 72(2) . . . . ?
Mn1 O4 Mo6' O33 -58(4) 1_655 . . . ?
Mo6 O4 Mo6' O31 -73.3(18) . . . 2_776 ?
Mn1 O4 Mo6' O31 156.4(18) 1_655 . . 2_776 ?
C44 C3 C6 C25 -3(3) . . . . ?
C44 C3 C6 C46 172(2) . . . . ?
O25 Mo4 O10 Mo4' 52(2) . . . . ?
O24 Mo4 O10 Mo4' -52.0(19) . . . . ?
O15 Mo4 O10 Mo4' 155.5(19) 1_455 . . . ?
O21 Mo4 O10 Mo4' -170(2) 1_455 . . . ?
O20 Mo4 O10 Mo4' -123.7(19) . . . . ?
O25 Mo4 O10 Mn1 -88.4(18) . . . . ?
O24 Mo4 O10 Mn1 167.9(17) . . . . ?
O15 Mo4 O10 Mn1 15.5(18) 1_455 . . . ?
O21 Mo4 O10 Mn1 50(3) 1_455 . . . ?
O20 Mo4 O10 Mn1 96.2(17) . . . . ?
O25 Mo4' O10 Mo4 -77(2) . . . . ?
O24 Mo4' O10 Mo4 83(2) . . . . ?
O25 Mo4' O10 Mn1 49(5) . . . . ?
O24 Mo4' O10 Mn1 -151(2) . . . . ?
O2 Mn1 O10 Mo4 -111.2(18) . . . . ?
O1 Mn1 O10 Mo4 -62(3) . . . . ?
O4 Mn1 O10 Mo4 62.2(18) 1_455 . . . ?
O1W Mn1 O10 Mo4 -18.8(17) . . . . ?
N1 Mn1 O10 Mo4 145.8(18) . . . . ?
O2 Mn1 O10 Mo4' 158(4) . . . . ?
O1 Mn1 O10 Mo4' -153(4) . . . . ?
O4 Mn1 O10 Mo4' -28(4) 1_455 . . . ?
O1W Mn1 O10 Mo4' -110(4) . . . . ?
N1 Mn1 O10 Mo4' 55(4) . . . . ?
O24 Mo5' O11 Mo5 -88(6) 2_675 . . . ?
O18 Mo5' O11 Mo5 64(3) . . . . ?
Mo3' Mo5' O11 Mo5 -20(4) . . . . ?
O18 Mo5 O11 Mo5' -63(4) . . . . ?
O17 Mo5 O11 Mo5' -165(4) . . . . ?
O24 Mo5 O11 Mo5' 39(4) 2_675 . . . ?
O19 Mo5 O11 Mo5' 122(4) . . . . ?
O20 Mo5 O11 Mo5' 96(4) 2_675 . . . ?
O1 Mo2' O14 Mo2 78(3) . . . . ?
O26 Mo2' O14 Mo2 -101.1(19) . . . . ?
O27 Mo2' O14 Mo2 -25.7(8) . . . . ?
O1 Mo2' O14 Mo6 -131(3) . . . . ?
O26 Mo2' O14 Mo6 50.1(11) . . . . ?
O27 Mo2' O14 Mo6 125.5(15) . . . . ?
O13 Mo2 O14 Mo2' -146.0(18) . . . . ?
O1 Mo2 O14 Mo2' -38.4(18) . . . . ?
O27 Mo2 O14 Mo2' 86(2) . . . . ?
O28 Mo2 O14 Mo2' 125.0(18) . . . . ?
O26 Mo2 O14 Mo2' 54.1(18) . . . . ?
O13 Mo2 O14 Mo6 -178.9(6) . . . . ?
O1 Mo2 O14 Mo6 -71.2(7) . . . . ?
O27 Mo2 O14 Mo6 52.9(11) . . . . ?
O28 Mo2 O14 Mo6 92.1(6) . . . . ?
O26 Mo2 O14 Mo6 21.2(5) . . . . ?
O33 Mo6 O14 Mo2' 44.3(12) . . . . ?
O4 Mo6 O14 Mo2' 150.4(12) . . . . ?
O31 Mo6 O14 Mo2' -88.9(14) 2_776 . . . ?
O26 Mo6 O14 Mo2' -40.5(11) . . . . ?
O32 Mo6 O14 Mo2' -114.1(11) 2_776 . . . ?
O33 Mo6 O14 Mo2 62.9(7) . . . . ?
O4 Mo6 O14 Mo2 169.0(6) . . . . ?
O31 Mo6 O14 Mo2 -70.2(10) 2_776 . . . ?
O26 Mo6 O14 Mo2 -21.8(5) . . . . ?
O32 Mo6 O14 Mo2 -95.5(6) 2_776 . . . ?
O16 Mo3 O15 Mo4 175.9(7) . . . 1_655 ?
O2 Mo3 O15 Mo4 67.0(7) . . . 1_655 ?
O17 Mo3 O15 Mo4 -57.4(12) . . . 1_655 ?
O19 Mo3 O15 Mo4 -94.2(6) . . . 1_655 ?
O21 Mo3 O15 Mo4 -21.9(5) . . . 1_655 ?
O19 Mo3' O16 Mo3 -104(9) . . . . ?
O17 Mo3' O16 Mo3 68(4) . . . . ?
Mo5' Mo3' O16 Mo3 150(5) . . . . ?
O2 Mo3 O16 Mo3' -152(3) . . . . ?
O15 Mo3 O16 Mo3' 105(3) . . . . ?
O17 Mo3 O16 Mo3' -50(3) . . . . ?
O19 Mo3 O16 Mo3' 22(3) . . . . ?
O21 Mo3 O16 Mo3' 45(4) . . . . ?
O11 Mo5 O17 Mo3 -67.6(7) . . . . ?
O18 Mo5 O17 Mo3 -174.6(7) . . . . ?
O24 Mo5 O17 Mo3 59.8(12) 2_675 . . . ?
O19 Mo5 O17 Mo3 20.1(5) . . . . ?
O20 Mo5 O17 Mo3 91.5(6) 2_675 . . . ?
O11 Mo5 O17 Mo3' -44.0(12) . . . . ?
O18 Mo5 O17 Mo3' -151.0(12) . . . . ?
O24 Mo5 O17 Mo3' 83.4(14) 2_675 . . . ?
O19 Mo5 O17 Mo3' 43.7(11) . . . . ?
O20 Mo5 O17 Mo3' 115.1(11) 2_675 . . . ?
O16 Mo3 O17 Mo5 67.8(7) . . . . ?
O2 Mo3 O17 Mo5 176.5(7) . . . . ?
O15 Mo3 O17 Mo5 -59.0(12) . . . . ?
O19 Mo3 O17 Mo5 -20.2(5) . . . . ?
O21 Mo3 O17 Mo5 -92.6(6) . . . . ?
O16 Mo3 O17 Mo3' 24.1(18) . . . . ?
O2 Mo3 O17 Mo3' 132.7(18) . . . . ?
O15 Mo3 O17 Mo3' -102.8(19) . . . . ?
O19 Mo3 O17 Mo3' -64.0(17) . . . . ?
O21 Mo3 O17 Mo3' -136.3(17) . . . . ?
O16 Mo3' O17 Mo5 133(4) . . . . ?
O19 Mo3' O17 Mo5 -50.5(10) . . . . ?
Mo5' Mo3' O17 Mo5 14.9(8) . . . . ?
O16 Mo3' O17 Mo3 -85(4) . . . . ?
O19 Mo3' O17 Mo3 91.4(17) . . . . ?
Mo5' Mo3' O17 Mo3 156.9(18) . . . . ?
O11 Mo5 O18 Mo5' 25(2) . . . . ?
O17 Mo5 O18 Mo5' 130(2) . . . . ?
O24 Mo5 O18 Mo5' -76(2) 2_675 . . . ?
O19 Mo5 O18 Mo5' -172(3) . . . . ?
O20 Mo5 O18 Mo5' -147(2) 2_675 . . . ?
O11 Mo5' O18 Mo5 -95(5) . . . . ?
O24 Mo5' O18 Mo5 68.4(16) 2_675 . . . ?
Mo3' Mo5' O18 Mo5 -39.2(13) . . . . ?
O21 Cr2 O19 Mo3' -1.5(17) . . . . ?
O21 Cr2 O19 Mo3' 178.5(17) 2_775 . . . ?
O20 Cr2 O19 Mo3' -86.5(17) 1_655 . . . ?
O20 Cr2 O19 Mo3' 93.5(17) 2_675 . . . ?
O19 Cr2 O19 Mo3' 169(86) 2_775 . . . ?
O21 Cr2 O19 Mo5 -95.0(4) . . . . ?
O21 Cr2 O19 Mo5 85.0(4) 2_775 . . . ?
O20 Cr2 O19 Mo5 -179.9(4) 1_655 . . . ?
O20 Cr2 O19 Mo5 0.1(4) 2_675 . . . ?
O19 Cr2 O19 Mo5 75(52) 2_775 . . . ?
O21 Cr2 O19 Mo3 1.2(4) . . . . ?
O21 Cr2 O19 Mo3 -178.8(4) 2_775 . . . ?
O20 Cr2 O19 Mo3 -83.7(4) 1_655 . . . ?
O20 Cr2 O19 Mo3 96.3(4) 2_675 . . . ?
O19 Cr2 O19 Mo3 172(52) 2_775 . . . ?
O16 Mo3' O19 Cr2 113(8) . . . . ?
O17 Mo3' O19 Cr2 -61.4(17) . . . . ?
Mo5' Mo3' O19 Cr2 -125.2(15) . . . . ?
O16 Mo3' O19 Mo5 -145(9) . . . . ?
O17 Mo3' O19 Mo5 40.9(8) . . . . ?
Mo5' Mo3' O19 Mo5 -22.9(8) . . . . ?
O16 Mo3' O19 Mo3 108(9) . . . . ?
O17 Mo3' O19 Mo3 -66.3(16) . . . . ?
Mo5' Mo3' O19 Mo3 -130(2) . . . . ?
O11 Mo5 O19 Cr2 -170.4(6) . . . . ?
O18 Mo5 O19 Cr2 26.6(19) . . . . ?
O17 Mo5 O19 Cr2 87.7(5) . . . . ?
O24 Mo5 O19 Cr2 -72.7(5) 2_675 . . . ?
O20 Mo5 O19 Cr2 -0.1(4) 2_675 . . . ?
O11 Mo5 O19 Mo3' 55.3(12) . . . . ?
O18 Mo5 O19 Mo3' -108(2) . . . . ?
O17 Mo5 O19 Mo3' -46.7(12) . . . . ?
O24 Mo5 O19 Mo3' 153.0(12) 2_675 . . . ?
O20 Mo5 O19 Mo3' -134.4(12) 2_675 . . . ?
O11 Mo5 O19 Mo3 86.6(5) . . . . ?
O18 Mo5 O19 Mo3 -76.5(18) . . . . ?
O17 Mo5 O19 Mo3 -15.3(4) . . . . ?
O24 Mo5 O19 Mo3 -175.7(5) 2_675 . . . ?
O20 Mo5 O19 Mo3 -103.1(4) 2_675 . . . ?
O16 Mo3 O19 Cr2 170.9(6) . . . . ?
O2 Mo3 O19 Cr2 -27.4(18) . . . . ?
O15 Mo3 O19 Cr2 71.0(5) . . . . ?
O17 Mo3 O19 Cr2 -89.8(5) . . . . ?
O21 Mo3 O19 Cr2 -1.1(4) . . . . ?
O16 Mo3 O19 Mo3' -13(2) . . . . ?
O2 Mo3 O19 Mo3' 149(2) . . . . ?
O15 Mo3 O19 Mo3' -113(2) . . . . ?
O17 Mo3 O19 Mo3' 87(2) . . . . ?
O21 Mo3 O19 Mo3' 175(2) . . . . ?
O16 Mo3 O19 Mo5 -84.3(5) . . . . ?
O2 Mo3 O19 Mo5 77.4(17) . . . . ?
O15 Mo3 O19 Mo5 175.9(5) . . . . ?
O17 Mo3 O19 Mo5 15.0(4) . . . . ?
O21 Mo3 O19 Mo5 103.7(4) . . . . ?
O25 Mo4 O20 Cr2 25.8(17) . . . 1_455 ?
O10 Mo4 O20 Cr2 -166.7(5) . . . 1_455 ?
O24 Mo4 O20 Cr2 92.1(5) . . . 1_455 ?
O15 Mo4 O20 Cr2 -74.8(4) 1_455 . . 1_455 ?
O21 Mo4 O20 Cr2 -0.8(4) 1_455 . . 1_455 ?
O25 Mo4 O20 Mo5 -77.5(16) . . . 2_675 ?
O10 Mo4 O20 Mo5 89.9(5) . . . 2_675 ?
O24 Mo4 O20 Mo5 -11.2(4) . . . 2_675 ?
O15 Mo4 O20 Mo5 -178.1(4) 1_455 . . 2_675 ?
O21 Mo4 O20 Mo5 -104.1(4) 1_455 . . 2_675 ?
O21 Cr2 O21 Mo4 116(23) 2_775 . . 1_655 ?
O20 Cr2 O21 Mo4 -0.9(4) 1_655 . . 1_655 ?
O20 Cr2 O21 Mo4 179.1(4) 2_675 . . 1_655 ?
O19 Cr2 O21 Mo4 82.2(5) 2_775 . . 1_655 ?
O19 Cr2 O21 Mo4 -97.8(5) . . . 1_655 ?
O21 Cr2 O21 Mo3 -147(23) 2_775 . . . ?
O20 Cr2 O21 Mo3 95.7(4) 1_655 . . . ?
O20 Cr2 O21 Mo3 -84.3(4) 2_675 . . . ?
O19 Cr2 O21 Mo3 178.8(4) 2_775 . . . ?
O19 Cr2 O21 Mo3 -1.2(4) . . . . ?
O16 Mo3 O21 Cr2 -23.4(17) . . . . ?
O2 Mo3 O21 Cr2 172.9(5) . . . . ?
O15 Mo3 O21 Cr2 -87.9(5) . . . . ?
O17 Mo3 O21 Cr2 74.4(5) . . . . ?
O19 Mo3 O21 Cr2 1.1(4) . . . . ?
O16 Mo3 O21 Mo4 81.4(16) . . . 1_655 ?
O2 Mo3 O21 Mo4 -82.2(5) . . . 1_655 ?
O15 Mo3 O21 Mo4 17.0(4) . . . 1_655 ?
O17 Mo3 O21 Mo4 179.3(4) . . . 1_655 ?
O19 Mo3 O21 Mo4 106.0(4) . . . 1_655 ?
O25 Mo4' O24 Mo4 88(5) . . . . ?
O10 Mo4' O24 Mo4 -57.2(18) . . . . ?
O25 Mo4' O24 Mo5 134(4) . . . 2_675 ?
O10 Mo4' O24 Mo5 -11(4) . . . 2_675 ?
O25 Mo4' O24 Mo5' -143(5) . . . 2_675 ?
O10 Mo4' O24 Mo5' 72(5) . . . 2_675 ?
O25 Mo4 O24 Mo4' -27(2) . . . . ?
O10 Mo4 O24 Mo4' 80(2) . . . . ?
O15 Mo4 O24 Mo4' -162(2) 1_455 . . . ?
O21 Mo4 O24 Mo4' -116(2) 1_455 . . . ?
O20 Mo4 O24 Mo4' 173(2) . . . . ?
O25 Mo4 O24 Mo5 176.6(7) . . . 2_675 ?
O10 Mo4 O24 Mo5 -76.0(8) . . . 2_675 ?
O15 Mo4 O24 Mo5 41.5(13) 1_455 . . 2_675 ?
O21 Mo4 O24 Mo5 87.7(7) 1_455 . . 2_675 ?
O20 Mo4 O24 Mo5 16.1(6) . . . 2_675 ?
O25 Mo4 O24 Mo5' -163(3) . . . 2_675 ?
O10 Mo4 O24 Mo5' -55(3) . . . 2_675 ?
O15 Mo4 O24 Mo5' 62(3) 1_455 . . 2_675 ?
O21 Mo4 O24 Mo5' 109(3) 1_455 . . 2_675 ?
O20 Mo4 O24 Mo5' 37(3) . . . 2_675 ?
O24 Mo4' O25 Mo4 -89(5) . . . . ?
O10 Mo4' O25 Mo4 55.7(16) . . . . ?
O10 Mo4 O25 Mo4' -79(2) . . . . ?
O24 Mo4 O25 Mo4' 27(2) . . . . ?
O15 Mo4 O25 Mo4' -175(2) 1_455 . . . ?
O21 Mo4 O25 Mo4' 114(2) 1_455 . . . ?
O20 Mo4 O25 Mo4' 88(3) . . . . ?
C48 N3 C25 C6 -2(3) . . . . ?
C3 C6 C25 N3 3(3) . . . . ?
C46 C6 C25 N3 -171.9(19) . . . . ?
O1 Mo2' O26 Cr1 -121(7) . . . . ?
O14 Mo2' O26 Cr1 57.9(19) . . . . ?
O27 Mo2' O26 Cr1 -58.5(17) . . . . ?
O1 Mo2' O26 Mo6 139(8) . . . . ?
O14 Mo2' O26 Mo6 -42.6(9) . . . . ?
O27 Mo2' O26 Mo6 -159.0(9) . . . . ?
O1 Mo2' O26 Mo2 -108(8) . . . . ?
O14 Mo2' O26 Mo2 70.6(19) . . . . ?
O27 Mo2' O26 Mo2 -45.8(16) . . . . ?
O28 Cr1 O26 Mo2' -171.2(18) 2_776 . . . ?
O28 Cr1 O26 Mo2' 8.8(18) . . . . ?
O26 Cr1 O26 Mo2' 130(100) 2_776 . . . ?
O32 Cr1 O26 Mo2' -88.1(18) 2_776 . . . ?
O32 Cr1 O26 Mo2' 91.9(18) . . . . ?
O28 Cr1 O26 Mo6 -80.5(5) 2_776 . . . ?
O28 Cr1 O26 Mo6 99.5(5) . . . . ?
O26 Cr1 O26 Mo6 -139(77) 2_776 . . . ?
O32 Cr1 O26 Mo6 2.6(5) 2_776 . . . ?
O32 Cr1 O26 Mo6 -177.4(5) . . . . ?
O28 Cr1 O26 Mo2 -177.8(4) 2_776 . . . ?
O28 Cr1 O26 Mo2 2.2(4) . . . . ?
O26 Cr1 O26 Mo2 123(77) 2_776 . . . ?
O32 Cr1 O26 Mo2 -94.7(4) 2_776 . . . ?
O32 Cr1 O26 Mo2 85.3(4) . . . . ?
O33 Mo6 O26 Mo2' -59.1(13) . . . . ?
O4 Mo6 O26 Mo2' 82(2) . . . . ?
O31 Mo6 O26 Mo2' -158.8(13) 2_776 . . . ?
O14 Mo6 O26 Mo2' 44.3(13) . . . . ?
O32 Mo6 O26 Mo2' 129.4(13) 2_776 . . . ?
O33 Mo6 O26 Cr1 169.2(6) . . . . ?
O4 Mo6 O26 Cr1 -49.5(18) . . . . ?
O31 Mo6 O26 Cr1 69.5(5) 2_776 . . . ?
O14 Mo6 O26 Cr1 -87.4(5) . . . . ?
O32 Mo6 O26 Cr1 -2.3(4) 2_776 . . . ?
O33 Mo6 O26 Mo2 -87.3(5) . . . . ?
O4 Mo6 O26 Mo2 54.0(17) . . . . ?
O31 Mo6 O26 Mo2 173.0(4) 2_776 . . . ?
O14 Mo6 O26 Mo2 16.1(4) . . . . ?
O32 Mo6 O26 Mo2 101.2(4) 2_776 . . . ?
O13 Mo2 O26 Mo2' -146(3) . . . . ?
O1 Mo2 O26 Mo2' 16(2) . . . . ?
O14 Mo2 O26 Mo2' -82(2) . . . . ?
O27 Mo2 O26 Mo2' 114(2) . . . . ?
O28 Mo2 O26 Mo2' -172(2) . . . . ?
O13 Mo2 O26 Cr1 24.7(15) . . . . ?
O1 Mo2 O26 Cr1 -173.8(5) . . . . ?
O14 Mo2 O26 Cr1 88.4(5) . . . . ?
O27 Mo2 O26 Cr1 -75.9(5) . . . . ?
O28 Mo2 O26 Cr1 -2.0(4) . . . . ?
O13 Mo2 O26 Mo6 -80.1(14) . . . . ?
O1 Mo2 O26 Mo6 81.4(5) . . . . ?
O14 Mo2 O26 Mo6 -16.4(4) . . . . ?
O27 Mo2 O26 Mo6 179.3(4) . . . . ?
O28 Mo2 O26 Mo6 -106.8(4) . . . . ?
O29 Mo1 O27 Mo2 71.2(7) . . . . ?
O30 Mo1 O27 Mo2 179.2(6) . . . . ?
O31 Mo1 O27 Mo2 -53.1(11) . . . . ?
O28 Mo1 O27 Mo2 -19.5(5) . . . . ?
O32 Mo1 O27 Mo2 -90.0(6) . . . . ?
O29 Mo1 O27 Mo2' 97.1(14) . . . . ?
O30 Mo1 O27 Mo2' -154.9(14) . . . . ?
O31 Mo1 O27 Mo2' -27.2(18) . . . . ?
O28 Mo1 O27 Mo2' 6.4(13) . . . . ?
O32 Mo1 O27 Mo2' -64.1(14) . . . . ?
O13 Mo2 O27 Mo1 -67.0(7) . . . . ?
O1 Mo2 O27 Mo1 -174.9(6) . . . . ?
O14 Mo2 O27 Mo1 60.9(11) . . . . ?
O28 Mo2 O27 Mo1 19.6(5) . . . . ?
O26 Mo2 O27 Mo1 90.7(6) . . . . ?
O13 Mo2 O27 Mo2' 155.3(18) . . . . ?
O1 Mo2 O27 Mo2' 47.3(18) . . . . ?
O14 Mo2 O27 Mo2' -76.9(19) . . . . ?
O28 Mo2 O27 Mo2' -118.2(18) . . . . ?
O26 Mo2 O27 Mo2' -47.0(18) . . . . ?
O1 Mo2' O27 Mo1 -147.8(14) . . . . ?
O26 Mo2' O27 Mo1 52.4(19) . . . . ?
O14 Mo2' O27 Mo1 -25(2) . . . . ?
O1 Mo2' O27 Mo2 -90(2) . . . . ?
O26 Mo2' O27 Mo2 110(2) . . . . ?
O14 Mo2' O27 Mo2 33.1(10) . . . . ?
O28 Cr1 O28 Mo2 91(100) 2_776 . . . ?
O26 Cr1 O28 Mo2 -2.3(4) . . . . ?
O26 Cr1 O28 Mo2 177.7(4) 2_776 . . . ?
O32 Cr1 O28 Mo2 82.5(4) 2_776 . . . ?
O32 Cr1 O28 Mo2 -97.5(4) . . . . ?
O28 Cr1 O28 Mo1 -171(100) 2_776 . . . ?
O26 Cr1 O28 Mo1 95.1(5) . . . . ?
O26 Cr1 O28 Mo1 -84.9(5) 2_776 . . . ?
O32 Cr1 O28 Mo1 179.8(4) 2_776 . . . ?
O32 Cr1 O28 Mo1 -0.2(4) . . . . ?
O13 Mo2 O28 Cr1 -168.1(6) . . . . ?
O1 Mo2 O28 Cr1 31.7(19) . . . . ?
O14 Mo2 O28 Cr1 -69.4(5) . . . . ?
O27 Mo2 O28 Cr1 90.7(5) . . . . ?
O26 Mo2 O28 Cr1 2.0(4) . . . . ?
O13 Mo2 O28 Mo1 86.3(5) . . . . ?
O1 Mo2 O28 Mo1 -73.9(18) . . . . ?
O14 Mo2 O28 Mo1 -175.0(4) . . . . ?
O27 Mo2 O28 Mo1 -14.9(4) . . . . ?
O26 Mo2 O28 Mo1 -103.6(4) . . . . ?
O29 Mo1 O28 Cr1 169.7(6) . . . . ?
O30 Mo1 O28 Cr1 -25.3(16) . . . . ?
O27 Mo1 O28 Cr1 -90.3(5) . . . . ?
O31 Mo1 O28 Cr1 73.0(5) . . . . ?
O32 Mo1 O28 Cr1 0.1(4) . . . . ?
O29 Mo1 O28 Mo2 -85.1(5) . . . . ?
O30 Mo1 O28 Mo2 79.9(14) . . . . ?
O27 Mo1 O28 Mo2 14.9(4) . . . . ?
O31 Mo1 O28 Mo2 178.2(4) . . . . ?
O32 Mo1 O28 Mo2 105.3(4) . . . . ?
O31 Mo1' O29 Mo1 70(3) . . . . ?
O30 Mo1' O29 Mo1 -55(2) . . . . ?
O30 Mo1 O29 Mo1' 58(3) . . . . ?
O27 Mo1 O29 Mo1' 159(3) . . . . ?
O31 Mo1 O29 Mo1' -46(3) . . . . ?
O28 Mo1 O29 Mo1' -128(3) . . . . ?
O32 Mo1 O29 Mo1' -96(3) . . . . ?
O29 Mo1 O30 Mo1' -33.9(18) . . . . ?
O27 Mo1 O30 Mo1' -137.5(18) . . . . ?
O31 Mo1 O30 Mo1' 66.9(18) . . . . ?
O28 Mo1 O30 Mo1' 162(2) . . . . ?
O32 Mo1 O30 Mo1' 137.9(17) . . . . ?
O29 Mo1' O30 Mo1 72(3) . . . . ?
O31 Mo1' O30 Mo1 -68.2(15) . . . . ?
O29 Mo1' O31 Mo6' 153(3) . . . 2_776 ?
O30 Mo1' O31 Mo6' -72(3) . . . 2_776 ?
O29 Mo1' O31 Mo6 -140(3) . . . 2_776 ?
O30 Mo1' O31 Mo6 -5(3) . . . 2_776 ?
O29 Mo1' O31 Mo1 -79(4) . . . . ?
O30 Mo1' O31 Mo1 56.0(13) . . . . ?
O29 Mo1 O31 Mo6' 138(3) . . . 2_776 ?
O30 Mo1 O31 Mo6' 30(3) . . . 2_776 ?
O27 Mo1 O31 Mo6' -97(3) . . . 2_776 ?
O28 Mo1 O31 Mo6' -130(3) . . . 2_776 ?
O32 Mo1 O31 Mo6' -58(3) . . . 2_776 ?
O29 Mo1 O31 Mo6 177.4(7) . . . 2_776 ?
O30 Mo1 O31 Mo6 69.6(7) . . . 2_776 ?
O27 Mo1 O31 Mo6 -57.5(12) . . . 2_776 ?
O28 Mo1 O31 Mo6 -89.7(6) . . . 2_776 ?
O32 Mo1 O31 Mo6 -18.3(6) . . . 2_776 ?
O29 Mo1 O31 Mo1' 30.1(18) . . . . ?
O30 Mo1 O31 Mo1' -77.7(18) . . . . ?
O27 Mo1 O31 Mo1' 155.2(19) . . . . ?
O28 Mo1 O31 Mo1' 122.9(18) . . . . ?
O32 Mo1 O31 Mo1' -165.6(18) . . . . ?
O28 Cr1 O32 Mo1 -179.8(4) 2_776 . . . ?
O28 Cr1 O32 Mo1 0.2(4) . . . . ?
O26 Cr1 O32 Mo1 -83.3(5) . . . . ?
O26 Cr1 O32 Mo1 96.7(5) 2_776 . . . ?
O32 Cr1 O32 Mo1 170(17) 2_776 . . . ?
O28 Cr1 O32 Mo6 85.9(4) 2_776 . . 2_776 ?
O28 Cr1 O32 Mo6 -94.1(4) . . . 2_776 ?
O26 Cr1 O32 Mo6 -177.6(4) . . . 2_776 ?
O26 Cr1 O32 Mo6 2.5(4) 2_776 . . 2_776 ?
O32 Cr1 O32 Mo6 76(17) 2_776 . . 2_776 ?
O29 Mo1 O32 Cr1 -33.5(17) . . . . ?
O30 Mo1 O32 Cr1 171.2(5) . . . . ?
O27 Mo1 O32 Cr1 73.3(5) . . . . ?
O31 Mo1 O32 Cr1 -87.7(5) . . . . ?
O28 Mo1 O32 Cr1 -0.1(4) . . . . ?
O29 Mo1 O32 Mo6 66.6(15) . . . 2_776 ?
O30 Mo1 O32 Mo6 -88.7(5) . . . 2_776 ?
O27 Mo1 O32 Mo6 173.4(4) . . . 2_776 ?
O31 Mo1 O32 Mo6 12.4(4) . . . 2_776 ?
O28 Mo1 O32 Mo6 99.9(4) . . . 2_776 ?
O31 Mo6' O33 Mo6 74(3) 2_776 . . . ?
O4 Mo6' O33 Mo6 -57.7(17) . . . . ?
O4 Mo6 O33 Mo6' 66(2) . . . . ?
O31 Mo6 O33 Mo6' -39(2) 2_776 . . . ?
O14 Mo6 O33 Mo6' 163(2) . . . . ?
O26 Mo6 O33 Mo6' -125(2) . . . . ?
O32 Mo6 O33 Mo6' -103(3) 2_776 . . . ?
C46 N4 C40 C40 84(3) . . . 2_566 ?
C50 N1 C43 C2 0(3) . . . . ?
Mn1 N1 C43 C2 -172.8(13) . . . . ?
C45 C2 C43 N1 1(3) . . . . ?
C51 C2 C43 N1 -175.2(17) . . . . ?
C6 C3 C44 C48 2(4) . . . . ?
C43 C2 C45 C49 0(3) . . . . ?
C51 C2 C45 C49 176.5(18) . . . . ?
C40 N4 C46 O23 -2(3) . . . . ?
C40 N4 C46 C6 175.0(16) . . . . ?
C25 C6 C46 O23 166.8(19) . . . . ?
C3 C6 C46 O23 -8(2) . . . . ?
C25 C6 C46 N4 -11(3) . . . . ?
C3 C6 C46 N4 174.2(19) . . . . ?
C3 C44 C48 N3 -1(4) . . . . ?
C25 N3 C48 C44 0(3) . . . . ?
C2 C45 C49 C50 -3(3) . . . . ?
C43 N1 C50 C49 -3(3) . . . . ?
Mn1 N1 C50 C49 169.5(14) . . . . ?
C45 C49 C50 N1 4(3) . . . . ?
C4 N2 C51 O22 2(3) . . . . ?
C4 N2 C51 C2 178.2(17) . . . . ?
C45 C2 C51 O22 -14(3) . . . . ?
C43 C2 C51 O22 162.3(18) . . . . ?
C45 C2 C51 N2 169.5(18) . . . . ?
C43 C2 C51 N2 -14(3) . . . . ?

_diffrn_measured_fraction_theta_max 0.980
_diffrn_reflns_theta_full        28.44
_diffrn_measured_fraction_theta_full 0.980
_refine_diff_density_max         3.940
_refine_diff_density_min         -2.212
_refine_diff_density_rms         0.407
